**Correlated-Electron Systems and High-Temperature **

**Superconductivity **

**Takashi Yanagisawa1, Mitake Miyazaki2, Kunihiko Yamaji1**

1_{Electronics and Photonics Research Group, National Institute of Advanced Industrial Science and Technology (AIST), }
Tsukuba Central 2, Tsukuba, Japan

2_{Hakodate National College of Technology, Hakodate, Japan }
Email: t-yanagisawa@aist.go.jp

Received April 2, 2013; revised May 5, 2013; accepted June 1,2013

Copyright © 2013 Takashi Yanagisawa *et al*. This is an open access article distributed under the Creative Commons Attribution Li-
cense, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

**ABSTRACT **

We present recent theoretical results on superconductivity in correlated-electron systems, especially in the two-
dimensional Hubbard model and the three-band d-p model. The mechanism of superconductivity in high-temperature
superconductors has been extensively studied on the basis of various electronic models and also electron-phonon
models. In this study, we investigate the properties of superconductivity in correlated-electron systems by using
numerical methods such as the variational Monte Carlo method and the quantum Monte Carlo method. The Hubbard
model is one of basic models for strongly correlated electron systems, and is regarded as the model of cuprate high
temperature superconductors. The d-p model is more realistic model for cuprates. The superconducting condensation
energy obtained by adopting the Gutzwiller ansatz is in reasonable agreement with the condensation energy estimated
for YBa2Cu3O7. We show the phase diagram of the ground state using this method. We have further investigated the
stability of striped and checkerboard states in the under-doped region. Holes doped in a half-filled square lattice lead to
an incommensurate spin and charge density wave. The relationship of the hole density *x* and incommensurability ,

*x*

, is satisfied in the lower doping region, as indicated by the variational Monte Carlo calculations for the
two-dimensional Hubbard model. A checkerboard-like charge-density modulation with a roughly 4 4 period has also
been observed by scanning tunneling microscopy experiments in Bi2212 and Na-CCOC compounds. We have
performed a variational Monte Carlo simulation on a two-dimensional *t*-*t*-*t*-*U* Hubbard model with a Bi-2212
type band structure and found that the 4 4 period checkerboard spin modulation, that is characterized by multi Q
vectors, is indeed stabilized. We have further performed an investigation by using a quantum Monte Carlo method,
which is a numerical method that can be used to simulate the behavior of correlated electron systems. We present a new
algorithm of the quantum Monte Carlo diagonalization that is a method for the evaluation of expectation value without
the negative sign problem. We compute pair correlation functions and show that pair correlation is indeed enhanced
with hole doping.

**Keywords:** High-Temperature Superconductivity; Strongly Correlated Electrons; Monte Carlo Methods; Hubbard

Model; Condensation Energy; Pair-Correlation Function

**1. Introduction **

The effect of the strong correlation between electrons is important for many quantum critical phenomena, such as unconventional superconductivity (SC) and the metal- insulator transition. Typical correlated electron systems are high-temperature superconductors [1-5], heavy fer- mions [6-9] and organic conductors [10]. The phase diagram for the typical high-Tc cuprates is shown in

**Figure 1 **[9]. It has a characteristics that the region of

antiferromagnetic order exists at low carrier concentra-

tions and the superconducting phase is adjacent to the antiferromagnetism.

In the low-carrier region shown in **Figure 2**, there is

the anomalous metallic region where the susceptibility
and 1*T*1 show a peak above *Tc* suggesting an existence
of the pseudogap. To clarify an origin of the anomalous
metallic behaviors is also a subject attracting many
physicists as a challenging problem.

It has been established that the Cooper pairs of high-*Tc *

**Figure 1. Phase diagram delineating the regions of super- **
**conductivity and antiferromagnetic ordering of the Cu2+**
**ions for the hole-doped La****2–x****SrxCuO4 and electron-doped **

**Nd****2–x****CexCuO****4–y**** systems. **

**Figure 2. Phase diagram showing the regions of non-Fermi **
**liquid and pseudogap metal for the hole-doped case. The **
**boundaries indicated in the figure are not confirmed yet. **

symmetry were provided for the electron-doped cuprates
Nd2–*x*Ce*x*CuO4 [13-15]. Thus it is expected that the
superconductivity of electronic origin is a candidate for
the high-*Tc* superconductivity. We can also expect that
the origin of *d*-wave superconductivity lies in the on-
site Coulomb interaction of the two-dimensional Hub-
bard model.

The antiferromagnetism should also be examined in correlated electron systems. The undoped oxide com- pounds exhibit rich structures of antiferromagnetic cor- relations over a wide range of temperature that are described by the two-dimensional quantum antiferro- magnetism [16-18]. A small number of holes introduced by doping are responsible for the disappearance of long-range antiferromagnetic order [19-24].

Recent neutron scattering experiments have suggested
an existence of incommensurate ground states with
modulation vectors given by *Qs*

###

2 ,###

and###

4 ,0###

*c*

*Q* (or *Qs*

###

, 2 ###

and###

0, 4###

*c*

*Q* ) where denotes the hole-doping ratio
[25]. We can expect that the incommensurate cor-

relations are induced by holes doped into the Cu-O plane in the underdoped region. A checkerboard-like charge-density modulation with a roughly 4 4 pe- riod has also been observed by scanning tunneling microscopy experiments in Bi2212 and Na-CCOC com- pounds.

Recently the mechanism of superconductivity in high- temperature superconductors has been extensively stu- died using various two-dimensional (2D) models of electronic interactions. Among them the 2D Hubbard model [26] is the simplest and most fundamental model. This model has been studied intensively using numerical tools, such as the Quantum Monte Carlo method [27-42], and the variational Monte Carlo method [24,43-50]. The two-leg ladder Hubbard model was also investigated with respect to the mechanism of high-temperature supercon- ductivity [51-59].

Since the discovery of cuprate high-temperature su- perconductors, many researchers have tried to explain the occurrence of superconductivity of these materials in terms of the two-dimensional (2D) Hubbard model. However, it remains matter of considerable controversial as to whether the 2D Hubbard model accounts for the properties of high-temperature cuprate superconductors. This is because the membership of the the two-dimen- sional Hubbard model in the category of strongly correlated systems is a considerable barrier to progress on this problem. The quest for the existence of a superconducting transition in the 2D Hubbard model is a long-standing problem in correlated-electron physics, and has been the subject of intensive study [35,36,38,46, 60,61]. In particular, the results of quantum Monte Carlo methods, which are believed to be exact unbiased me- thods, have failed to show the existence of super- conductivity in this model [38,61].

In the weak coupling limit we can answer this question.
We can obtain the superconducting order parameter of
the Hubbard model in the limit of small *U*, that is given
by [62-66]

2 2

exp ,

*xU*

_{} _{}

(1)

where *U* is the strength of the on-site Coulomb
interaction and the exponent *x* is determined by solv-
ing the gap equation. Thus the existence of the super-
conducting gap is guaranteed by the weak coupling
theory although is extremely small because of the
exponential behavior given above. *x* indicates the
strength of superconductivity. In the intermediate or
large coupling region, we must study it beyond the
perturbation theory.

obtained by using the quantum variational Monte Carlo method. The superconducting condensation energy ob- tained by adopting the Gutzwiller ansatz is in reasonable agreement with the condensation energy derived for YBa2Cu3O7. We have further investigated the stability of striped and checkerboard states in the under-doped region. Holes doped in a half-filled square lattice lead to an incommensurate spin and charge density wave. The relationship of the hole density x and incommensurability

, *x*, is satisfied in the lower doping region. This
is consistent with the results by neutron scattering
measurements. To examine the stability of a 4 4

checkerboard state, we have performed a variational Monte Carlo simulation on a two-dimensional

*t t* *t* *U* Hubbard model with a Bi-2212 type band
structure. We found that the 4 4 period checkerboard
checkerboard spin modulation that is characterized by
multi *Q* vectors is stabilized.

Further investigation has been performed by using the quantum Monte Carlo method which is a numerical method that can be used to simulate the behavior of correlated electron systems. This method is believed to be an exact unbiased method. We compute pair cor- relation functions to examine a possibility of super- conductivity.

The Quantum Monte Carlo (QMC) method is a numerical method employed to simulate the behavior of correlated electron systems. It is well known, however, that there are significant issues associated with the application to the QMC. First, the standard Metropolis (or heat bath) algorithm is associated with the negative sign problem. Second, the convergence of the trial wave function is sometimes not monotonic, and further, is sometimes slow. In past studies, workers have inves- tigated the possibility of eliminating the negative sign problem [37,38,40-42]. We present the results obtained by a method, quantum Monte Carlo diagonalization, without the negative sign problem.

**2. Hubbard Hamiltonian **

The Hubbard Hamiltonian is
† _{,}

*ij i* *i* *i* *i*

*ij* *i*

*H*

###

*t c c*

*U*

###

*n n* (2)

where †

*i*

*c*_{} and *ci* denote the creation and annihilation

operators of electrons, respectively, and †

*i* *i* *i*

*n*_{} *c c*_{ } is
the number operator. The second term represents the
on-site Coulomb interaction which acts when the two
electrons occupy the same site. The numbers of lattice
sites and electrons are denoted as *N* and *Ne* ,

respectively. The electron density is *ne**N Ne* .

In the non-interacting limit *U*0, the Hamiltonian is
easily diagonalized in terms of the Fourier transformation.
In the ground state each energy level is occupied by

electrons up to the Fermi energy. In the other limit 0

*ij*

*t* , each site is occupied by the up- or down-spin
electron, or is empty. The non-zero *tij* induces the

movement of electrons that leads to a metallic state id

*e*

*N* *N* . The ground state is probably insulating at
half-filling *Ne**N* if *U* is sufficiently large.

If *tij* *t* are non-zero only for the nearest-neighbor

pairs, the Hubbard Hamiltonian is transformed to the
following effective Hamiltonian for large *U t* [67]:

2

† † †

† † † †

† † _{,}

*i* *j* *j* *j* *j*

*ij*

*j* *j* *j* *j* *j* *j* *j* *j*

*j* *j* *j* *j*

*t*

*H* *t* *a a* *a* *a a a*

*U*

*a a* *a* *a* *a* *a a* *a*

*a a* *a a*

_{}

_{}

###

###

(3)

where *ai* *ci*

###

1*ni*,

###

and*j* and

*j* in-

dicate the nearest-neighbor sites in the and
directions, respectively. The second term contains the
three-site terms when . If we neglect the three-site
terms, this effective Hamiltonian is reduced to the *t-J* model:

###

†_{h.c.}

###

1_{,}

4

*i* *j* *i* *j* *i* *j*

*ij* *ij*

*H* *t* *a a* *J* *n n*

_{} _{}

###

###

**S S**where _{J}_{}_{4}* _{t U}*2

_{. }

The Hubbard model has a long history in describing the magnetism of materials since the early works by Hubbard [26], Gutzwiller [68] and Kanamori [69]. One- dimensional Hubbard model has been well understood by means of the Bethe ansatz [70-72] and conformal field theory [73-75]. The solutions established a novel concept of the Tomonaga-Luttinger liquid [76] which is described by the scalar bosons corresponding to charge and spin sectors, respectively. The correlated electrons in two- and three-dimensional space are still far from a complete understanding in spite of the success for the one-di- mensional Hubbard model. A possibility of supercon- ductivity is a hot topic as well as the magnetism and metal-insulator transition for the two- and three-di- mensional Hubbard model.

The three-band Hubbard model that contains *d* and

*p* orbitals has also been investigated intensively with
respect to high temperature superconductors [24,64,
77-88]. This model is also called the *d-p *model. The 2D
three-band Hubbard model is the more realistic and
relevant model for two-dimensional CuO2 planes which
are contained usually in the crystal structures of high-*Tc*

superconductors. The network of CuO2 layer is shown in

**Figure 3**. The parameters of the three-band Hubbard

model are given by the Coulomb repulsion *Ud*, energy

levels of *p* electrons *p* and *d* electron *d*, and

transfer between *p* orbitals given by *tpp*. Typical

**Figure 3. The lattice of the three-band Hubbard model on **
**the CuO2 plane. Small circles denote Cu sites and large ones **

**denote O sites. **

**Table 1. Typical parameter values for the three-band Hub- **
**bard model. Energies are measured in eV. **

Ref.[90] Ref.[89] Ref.[91] Ref.[78]

*p* *d*

3.6 2.75 - 3.75 3.5 2.5

*dp*

*t* 1.3 1.5 1.5 1.47

*pp*

*t* 0.65 0.65 0.6

*d*

*U* 10.5 8.8 9.4 9.7

*p*

*U* 4.0 6.0 4.7 5.7

*dp*

*U* 1.2 <1.0 0.8 <1

three-band Hubbard model is written as [24,47,48,80] (see
Equation (4)) where ˆ*x* and ˆ*y* represent unit vectors
along *x* and *y * directions, respectively. †

ˆ 2,
*i x*

*p* and

ˆ 2,
*i x*

*p* denote the operators for the *p* electrons at site

ˆ 2

*i*

*R* *x* . Similarly †
ˆ 2,
*i y*

*p* and *pi y*ˆ 2, are defined.

*d*

*U* denotes the strength of Coulomb interaction between

*d* electrons. For simplicity we neglect the Coulomb
interaction among *p* electrons in this paper. Other
notations are standard and energies are measured in *tdp*

units. The number of cells is denoted as *N* for the
three-band Hubbard model. In the non-interacting case

###

*U*0

_{d}###

the Hamiltonian in the*k*-space is written as (see Equation (5)).

where *d k*

_{}

###

†

*d k*

_{},

*px*

**k**###

†

*x*

*p k*

_{}and

*py*

**k**###

†

*y*
*p* **k**_{}
are operators for *d* -, *px*- and *py* -electron of the

momentum * k* and spin , respectively.

In the limit *tdp**Ud*

###

*p*

*d*

###

,*tdp*

*p*

*d*, and

*p*

*d*

*Ud*

, the *d*- *p* model is mapped to the *t-J *

model with

###

###

2 1 2

4 ,

2

*eff*

*d* *p* *d* *p*

*J* *t*
*U* *U*
(6)

where 2

###

###

*eff* *dp* *p* *d*

*t* *t* . *JK* 4*teff* gives the

antiferromagnetic coupling between the neighboring *d*

and *p* electrons. In real materials

###

*p*

*d*

###

*tdp*is not

so large. Thus it seems that the mapping to the *t-J* model
is not necessarily justified.

**3. Variational Monte Carlo Studies **

In this Section we present studies on the two-dimensional Hubbard model by using the variational Monte Carlo method.

**3.1. Variational Monte Carlo Method **

Let us start by describing the method based on the 2D Hubbard model. The Hamiltonian is given by

###

###

###

###

† † h.c. h.c. ,*i*

*j*

*ij*

*j* *j* *j*

*j*
*j*

*H* *t* *c c*

*t* *c c* *U* *n n*

###

###

###

(7)where *ij* denotes summation over all the nearest-
neighbor bonds and *j* means summation over the
next nearest-neighbor pairs. *t* is our energy unit. The
dispersion is given by

###

###

###

###

###

###

2 cos*t* *kx* cos *ky* 4 cos*t* *kx* cos *ky* .

**k**

(8)

Our trial wave function is the Gutzwiller-projected wave functions defined as

0,

*e*

*n* *P PN* *G*

(9)

,

*e*

*s* *P PN* *G* *BCS*

(10)

###

###

###

###

† † † † †

ˆ/ 2, ˆ/ 2, ˆ/ 2, ˆ/ 2, †

ˆ/ 2, ˆ/ 2, ˆ/ 2, ˆ/ 2,

† † †

ˆ/ 2, ˆ/ 2, ˆ/ 2, ˆ/ 2, ˆ/ 2, ˆ/ 2 h.c.

*dp* *d* *i* *i* *d* *i* *i* *i* *i* *p* *i x* *i x* *i y* *i y*

*i* *i* *i*

*dp* *i* *i x* *i y* *i x* *i y*

*i*

*pp* *i y* *i x* *i y* *i x* *i y* *i x*

*H* *d d* *U* *d d d d* *p* *p* *p* *p*

*t* *d* *p* *p* *p* *p*

*t* *p* *p* *p* *p* *p* *p*

_{} _{}

###

###

###

###

† ˆ ˆ, *i y*/ 2, *i x*/ 2, h.c. .
*i*
*p* *p*

###

(4)###

###

###

###

###

###

###

###

###

###

###

###

###

###

###

###

###

###

0 ? † †2i sin 2 h.c.

2i sin 2 h.c. 4 sin 2 sin 2 h.c. ,

*dp* *d* *p* *x* *x* *y* *y* *dp* *x* *x*

*dp* *y* *y* *pp* *x* *y* *x* *y*

*H* *d d* *p* *p* *p* *p* *t* *k* *d p*

*t* *k* *d p* *t* *k* *k* *p* *p*

###

###

###

###

###

**k****k****k****k****k****k****k****k**

**k****k****k**

**k****k****k****k**

**k****k**

(5)

where
†
0
,
0 ,
*F*
*k*
*c*_{}

###

**k**

**k**(11)

###

† †###

_{0 .}

*BCS* *u* *v c c*

###

**

**k**

**k k**_{ }

**k**

**k**(12)

*G*

*P* is the Gutzwiller projection operator given by

###

###

1 1 ;

*G* *j* *j*

*k*

*P*

###

_{}

*g n n*

_{}

_{}

_{}(13)

*g* is a variational parameter in the range from 0 to unity
and *j* labels a site in the real space. *PN _{e}* is a pro-

jection operator which extracts only the sites with a fixed
total electron number *Ne*. Coefficients *u k* and

*v*in

**k***BCS*

appear in the ratio defined by

###

_{2}

_{2}

###

1 2,*v*

*u* _{} _{}

**k****k**

**k**

**k****k****k**

(14)

where *_{k}*

* and *

_{k}*is a*

_{k}*k*-dependent gap func- tion. is a variational parameter working like the chemical potential.

*c* is the Fourier transform of

**k***cj*.

The wave functions * _{n}* and

*are expressed by the Slater determinants for which the expectations values are evaluated using a Monte Carlo procedure [43,44,92]. *

_{s}*is written as*

_{s}###

###

###

###

† † † † 2 † † exp 0exp , 0

, 0 ,

*e*

*e*

*e*

*s* *N* *G*

*N* *G* *j*

*j*

*N*

*G* *j*

*j*

*P P* *v u c c*

*P P* *a j* *c c*

*P* *a j* *c c*

_{ }
_{} _{}
_{} _{}
_{} _{}

###

###

###

**k****k****k****k**

* k*
(15)
where

###

, 1###

###

###

exp###

*j*

###

.*a j* *N*

###

*v u*

_{k}**

_{k}_{}

*i*

_{}

**k**

**k****R**_{} **R**

(16)

Then * _{s}* is written using the Slater determinants as

###

###

1 2 1 2

1 2 2 1 2 2

1 2 1 2

† † † † † †

, 0 ,

*e* *e*

*Ne* *Ne*

*Ne* *Ne*

*s* *G* *N* *N*

*j* *j*

*j* *j* *j*

*P* *A j* *i*

*c c* *c* *c c* *c*

###

(17)where *A j*

###

1*iNe*2, 1

*Ne*2

###

is the Slater determinant defined by###

###

###

###

###

###

###

###

###

###

###

###

###

###

###

###

###

###

###

1 21 1 1 2 1 2

2 1 2 2 2 2

2 1 2 2 2 2

, , ,
, , ,
.
, , ,
*e*
*e*
*e*

*e* *e* *e* *e*

*N*

*N*

*N*

*N* *N* *N* *N*

*A j*

*a j* *a j* *a j*

*a j* *a j* *a j*

*a j* *a j* *a j*

(18)

In the process of Monte Carlo procedure the values of cofactors of the matrix in Equation (18) are stored and corrected at each time when the electron distribution is modified. We optimized the ground state energy

*g* *s* *s* *s* *s*

*E* *H* *H* (19)
with respect to *g*, *_{k}* and for

*s*for

*s*. For

*n*

the variational parameter is only *g* . We can
employ the correlated measurements method [93] in the
process of searching optimal parameter values mini-
mizing *Eg*.

A Monte Carlo algorithm developed in the auxiliary field quantum Monte Carlo calculations can also be employed in evaluating the expectation values for the wave functions shown above [94-96]. Note that the Gutzwiller projection operator is written as

exp ,

*G* *i* *i*

*i*
*P* _{} *n n*_{ }_{}

###

(20) where log 1###

*g*. Then using the discrete Hubbard- Stratonovich transformation, the Gutzwiller operator is the bilinear form:

###

###

###

###

###

exp

1 2 exp 2 ,

2

*i*
*i* *i*
*i*

*N*

*i* *i* *i* *i* *i*

*s* *i* *i*

*n n*

*a* *s n* *n* *n* *n*

_{}
_{} _{}

###

###

###

###

(21) where_{cosh 2}

###

_{a}_{}

_{e}2

_{. The Hubbard-Stratonovich au- }xiliary field

*si*takes the values of 1. The norm

*n* *n*

is written as

###

###

###

###

###

###

###

###

###

###

† 0 0const det exp ,

exp , ,

*i* *i*
*n* *n*
*u* *s*
*V* *u*
*V* *s*

###

(22)where *V*

###

*s*, is a diagonal

*N N* matrix corre- sponding to the potential

###

2 .2

*i i* *i*

*i* *i*

*h s* *a* *s n* *n*

###

###

(23)###

,*V* *s* is written as

###

, diag 2###

1 2, ,2*N*2,0,

###

,*V* *s* *a s* *a s*
(24)
where diag ,

###

*a*

###

denotes a diagonal matrix with ele- ments given by the arguments*a*,. The elements of

###

0

_{ij}

###

*i*1, , ;

*N j*1, ,

*N*2

_{e}###

are given by linear combinations of plane waves. For example,###

0*exp*

_{ij}###

*ii*

*j*

###

.

method is used to consider an off-diagonal Jastrow cor-
relation factor of exp(–*S*)-type. The results for the im-
proved wave functions are discussed in Section 3.10.

**3.2. Superconducting Condensation Energy **

We study the cases of the *d*-, extended *s*- (*s*-) and

*s*-wave gap functions in the following:

###

###

###

###

cos *x* cos *y* ,

*d* _{k}*k* *k* (26)

###

###

###

###

cos * _{x}* cos

*,*

_{y}*s* _{ } *k* _{} *k*

* k* (27)

.

*s* *_{k}* (28)
In

**Figure 4**calculated energies per site with

*Ne*84

on the 10 10 lattice are shown for the case of *U*8
and *t* 0[46]. *E Ng* is plotted as a function of

for three types of gap functions shown above. We impose the periodic and the antiperiodic boundary conditions for

*x*- and *y*-direction, respectively. This set of boundary
conditions is chosen so that *_{k}* does not vanish for any

*k*-points occupied by electrons. *Eg* was obtained as the

average of the results of several Monte Carlo calculations
each with _{5 10}_{} 7_{ steps. }

*g*

*E N* has minimum at a
finite value of 0.08 in the case of the *d*-wave gap
function.

The energy gain *Eg* in the superconducting state is

called the SC condensation energy in this paper.

*g*
*E N*

is plotted as a function of 1 *N* in **Figure 5** in

order to examine the size dependence of the SC energy gain [97]. Lattice sizes treated are from 8 8 to

22 22 . The electron density *ne* is in the range of

0.80*ne*0.86. Other parameters are 0.20 *t* 0.0
and *U t*8 in *t* units. Bulk limit *N* of SC
condensation energy *Econd* was obtained by plotting as

a function of 1*N*. The linear fitting line indicates very

**Figure 4. Ground state energy per site ****E****g****N for the 2D ****Hubbard model is plotted against **** for the case of 84 **
* electrons on the 10 × 10 lattice with U*

**8 and**

**

**t****0 .**

**Solid curves are for the d-wave gap function. Squares and**

**triangles are for the s*******

**- and s-wave gap functions,****respectively. The diamond shows the normal state value**

**[46].**

**Figure 5. Energy gain per site in the SC state with reference **
**to the normal state for the 2D Hubbard model is plotted as **
**a function of 1****N****. L is the length of the edge of the square ****lattice. YBCO attached to the vertical axis indicates the **
**experimental value of the SC condensation energy for **
**YBa2Cu3O4 [97]. **

clearly that the bulk limit remains finite when
0.25 *t* 0.10

and *n _{e}*0.84 . When

*n*0.86 , 0.20

_{e}*t* and *U*8 , the bulk-limit *E _{cond}* is
0.00117 site 0.60 meV site

*cond*

*E* , where *t* = 0.51

eV is used [98]. Thus the superconductivity is a real bulk
property, not a spurious size effect. The value is re-
markably close to experimental values 0.17 ~ 0.26
meV/site estimated from specific heat data [99,100] and
0.26 meV/site from the critical magnetic field *H _{c}* [101]
for optimally doped YBa2Cu3O4 (YBCO). This good
agreement strongly indicates that the 2D Hubbard model
includes essential ingredients for the superconductivity in
the cuprates.

We just point out that the *t-J* model gives
= 0.026 13 meV site

*cond*

*E* *t* at *n _{e}*0.84 for

*J*= 4

*t*2_{/}_{U}_{ = 0.5 and } _{t}_{ }_{0}_{ [102]. This value is 50 times larger }
than the experimental values indicating a serious quan-
titative problem with this model. This means that the *t-J *

model made from the leading two terms in the expansion
in terms of *t U* of the canonical transformation of the
Hubbard model should be treated with the higher-order
terms in order to give a realistic SC condensation ener-
gy.

Here we show the SC condensation energy as a
function of *U* in **Figure 6**. The condensation energy

*cond*

*E* *E N* is increased as *U t* is increased as far
as *U t*12. In the strong coupling region *U*8*t*, we
obtain the large condensation energy.

**3.3. Fermi Surface and Condensation Energy **

**Figure 6. Energy gain per site in the SC state with reference **
**to the normal state for the 2D Hubbard model as a function **
**of the Coulomb repulsion U. The system is 10 × 10 with the ****electron number ** * Ne*

**84 and**

* *

**t****0.3 .**

for YBCO. [103] The band parameter values of LSCO
were estimated as *t* 0.12 and *t* 0.08[104]. This
set corresponds roughly to *Econd* 0.0010. The latter
value is much larger than the above-mentioned experi-
mental value for LSCO. However, the stripe-type SDW
state coexists with superconductivity [105,106] and the
SC part of the whole *Econd* is much reduced. Therefore,

such a coexistence allows us to qualitatively understand
the SC *Econd* in LSCO.

On the other hand, Tl2201

###

*T*93 K

_{c}###

and Hg1201###

*Tc*98 K

###

band calculations by Singh and Pickett [107]give very much deformed Fermi surfaces that can be
fitted by large *t* such as *t* 0.4. For Tl2201, an
Angular Magnetoresistance Oscillations (AMRO) work
[108] gives information of the Fermi surface, which
allows to get *t* 0.2 and *t*0.165. There is also
an Angle-Resolved Photoemission Study (ARPES) [109],
which provides similar values. In the case of Hg1201,
there is an ARPES work [110], form which we obtain by
fitting *t* 0.2 and *t*0.175. For such a deformed
Fermi surface, *E _{cond}* in the bulk limit is reduced con-
siderably. [111,112] Therefore, the SC

*Econd*calculated

by VMC indicates that the Fermi surface of LSCO-type
is more favorable for high *Tc*. The lower *Tc* in LSCO

may be attributed to the coexistence with antiferro- magnetism of stripe type.

**3.4. Ladder Hubbard Model **

The SC condensation energy in the bulk limit for the ladder Hubbard model has also been evaluated using the variational Monte Carlo method [54]. The Hamiltonian is given by the 1D two-chain Hubbard model: [51,52,55, 56,85,113-116]

###

###

2###

###

† †

1 2 , 1,

1 2

† †

0 1

h.c. h.c.

,

*ladder* *d* *j* *j*

*j*

*j* *j* *j* *j*

*j*

*H* *t* *c c* *t* *c c*

*U* *c c c c*

###

###

###

(29)

where †
*j*

*c*_{}_{}

###

*c*

_{j}_{}

_{}is the creation (annihilation) operator of an electron with spin at the th site along the

*j*th chain

###

*j*1,2

###

.*t*is the intrachain nearest-neighbor transfer and

*td*is the interchain

nearest-neighbor transfer energy. The energy is measured
in *t* units. The energy minimum was given when the
components of the gap function *k* take finite values

plotted in **Figure 7** for the lattice of 20 2 sites with 34

electrons imposing the periodic boundary condition [54].
Each component of *k* was optimized for *U*08 and

1.8

*d*

*t* . There are two characteristic features; one is that
the components of the bonding and antibonding bands
have opposite signs each other and second is that the
absolute values of * _{k}* of the antibonding band

###

*ky*

###

is much larger than that of the bonding band###

*ky*0

###

. In order to reduce the computation cpu time,*k*

of each band was forced to take a fixed value
specific to each band, *i.e.* 1 for the bonding band and

2

for the antibonding band. This drastically reduces the number of the variational parameters but still allows us to get a substantial value of the condensation energy.

1

and 2 take opposite sign, which is similar to that
of the *d _{x}*2

_{}

*2 gap function.*

_{y}The energy gain *F*2*c* remains finite in the bulk limit

when 1.2 *t _{d}* 1.6. The SC condensation energy per
site in the bulk limit is plotted as a function of

*td*in

**Figure 8 **[54]. The SC region derived from the SC

condensation energy in the bulk limit is consistent with
the results obtained from the density-matrix renormali-
zation group [55,56] and the exact-diagonalization
method [51,52,115]. The maximum value of *E*2*c* is

0.0008 which is of the same order of magnitude as the maximum condensation energy obtained for the 2D Hubbard model [46].

**Figure 7. The values of components of ****k**** for the two- **
**chain Hubbard model. All the values of ****k of the bonding **_{x}**band **

###

**

**k**_{y}**0 and antibonding band**

###

###

* *

**k**_{y}###

**corre-**

**spond to the energy minimum for 20 × 2 lattice with 34**

**electrons. The parameters in the Hamiltonian are**

**

**t****d****1.8**

**and**

**U****0**

**8**

**and the variational parameters are**

**0.0182**

**Figure 8. ****t dependence of the SC condensation energy **_{d}

**E****N**

**2** ** for the two-chain Hubbard model in the bulk **
**limit [54].**

**3.5. Condensation Energy in the d-p Model **

The SC energy gain for the *d-p* model, namely, three-
band Hubbard model in Equation (4) has also been evalu-
ated using the variational Monte Carlo method. For the
three-band model the wave functions are written as

† ,

0 ,

*F*

*n* *G* *k*

*k k*

*P*

###

(30)###

† †###

_{0 ,}

*e*

*SC* *G N* *k* *k* *k* *k*

*k*

*P P* *u* *v*

###

_{ }(31) where

*k* is the linear combination of

*dk* ,

*pxk* and

*yk*

*p* _{} constructed to express the operator for the lowest
band (in the hole picture) or the highest band (in the
electron picture) of the non-interacting Hamiltonian. The
numerical calculations have been done in the hole picture.
The Gutzwiller parameter *g*, effective level difference

*p* *d*

, chemical potential and superconducting or- der parameter are the variational parameters.

The similar results to the single-band Hubbard model
were obtained as shown in **Figure 9** for *t _{pp}* 0.0,

8

*d*

*U* and *d**p*2 in *tdp* units where the cal-

culations were performed in the hole picture [24]. The SC condensation energy for the three-band model is

0.0005 0.75

*cond* *dp*

*E* *t* meV per site in the optimally
doped region. We set *tdp*1.5 eV as estimated in **Table **

**1**. There is a tendency that *Econd* increases as *d**p*

increases which is plotted in **Figure 10**. This tendency is

not, however, in accordance with NQR (nuclear quad- rupole resonance) study on cuprates. [117] We think that the NQR experiments indicate an importance of the Coulomb interaction on oxygen sites. This will be dis- cussed in Section 3.11.

**3.6. Antiferromagnetic State **

When the density of doped holes is zero or small, the 2D single-band or three-band Hubbard model takes an anti- ferromganetic state as its ground state. The magnetic

**Figure 9. Ground-state energy per site as a function of **
**with the d-wave gap function for the three-band Hubbard *** model. The size of lattice is 6 × 6. Parameters are U*

**8 ,**

**pp**

* t*

**0 and **

**

**p******

**

**d****2 in units of**

**t . The doping rate is****dp****0.111**

** for (a) and ****0.333 for (b). Squares denote **
**the energies for the normal-state wave function [24].**

**Figure 10. Energy gain per site in the SC state as a function **
**of the level difference ** **dp******* p*

****

**d****for the three-band**

**Hubbard model with**

**

**U**_{d}**8 and**

**

**t**_{pp}**0.2 [24]. The size**

**of lattice is 6 × 6 sites.**

order is destroyed and superconductivity appears with the
increase of doped hole density. The transition between
the *d*-wave SC and the uniform SDW states has been
investigated by computing the energy of the SDW state
by using the variational Monte Carlo method. The trial
SDW wave function is written as

,

*AF* *PG* *SDW*

###

† †###

† †###

_{0 ,}

*SDW* *u c* *v c* *Q* *u c* *v c* *Q*

###

_{k}**

_{k}

_{k}**

_{k}###

_{k}**

_{k}

_{k}

_{k}**k****k**

(33)

###

###

##

_{1 2}

##

1 2 2 21 * _{AF}* 2 ,

*u* _{} *w* *w* _{}

**k****k*** k* (34)

###

###

##

_{1 2}

##

1 2 2 21 * _{AF}* 2 ,

*v* _{} *w* *w* _{}

**k****k*** k* (35)

###

###

2.*k* *Q*

*w* * k*

* (36)*

**k**Summation over * k* and

* in Equation (33) is performed over the filled*

**k***k*-points, as in the calculation of the normal state energy.

*Q*is the SDW wave vector given by

###

, and *is the SDW potential am- plitude.*

_{AF}As shown in** Figure 11**, the energy gain per site in the

SDW state rises very sharply from *n _{e}*0.84 for

*t* 0

[46]. At *ne*0.84 it is slightly larger than that in the

SC state, and at *ne*0.80 there is no more stable SDW

state. Thus the boundary between the SDW and the SC
states is given at *n _{e}*0.84. The results of the bulk limit
calculations indicate that the energy gain in the SC state
at

*ne*0.84 takes the extremely small value and the

value at *n _{e}*0.80 vanishes as

*N*0. Hence the pure

*d*-wave SC state possibly exists near the boundary at

0.84

*e*

*n* , but the region of pure SC state is very
restricted.

Let us turn to the three-band model. We show the
antiferromagnetic-paramagnetic boundary for *tpp*0.0

and *p* *d* 2 in the plane of *U* and the hole density

in **Figure 12** where AF denotes the antiferromagnetic

region [47]. The value *p* *d* 2 is taken from the

estimations by cluster calculations [89-91]. The phase
boundary in the region of small *U* is drawn from an
extrapolation. For the intermediate values of *U*8 -12,

**Figure 11. Energy gain per site in the SDW state (diamonds) **
**against electron density for *** t*

**0 and the energy gain in**

**the SC state for**

**

**t****0 (open circles) and**

* *

**t****0.1 (solid**

**circles). The model is the 2D Hubbard model on 10 × 10**

**lattice [46].**

**Figure 12. Antiferromagnetic region in the plane of U and ****the hole density for ** * tpp*

**0.0 and **

**

**p******

**

**d****2.**

the antiferromagnetic long-range ordering exists up to about 20 percent doping. Thus the similar features are observed compared to the single-band Hubbard model.

Since the three-band Hubbard model contains several
parameters, we must examine the parameter dependence
of the energy of SDW state. The energy gain *ESDW* in

the SDW state is shown in **Figure 13** as a function of

doping ratio for several values of *dp* *p**d*. *ESDW*

increases as *dp* increases as expected. In **Figure 14**
*pp*

*t* - and *Ud* -dependencies of *ESDW* are presented.

The SDW phase extends up to 30 percent doping when

*d*

*U* is large. It follows from the calculations that the
SDW region will be reduced if *p**d* and *Ud* de-

crease.

From the calculations for the SDW wave functions, we
should set *p**d* and *Ud* small so that the SDW

phase does not occupy a huge region near half-filling. In

**Figures 15** and **16**, we show energy gains for both the

SDW and SC states for *Ud*8, *tpp*0, 0.2 and

2

*p* *d*

, where the right hand side and left hand side indicate the hole-doped and electron-doped case, res- pectively. Solid symbols indicate the results for 8 8

and open symbols for 6 6 . For this set of parameters
the SDW region extends up to 20 percent doping and the
pure *d*-wave phase exists outside of the SDW phase. The

*d*-wave phase may be possibly identified with supercon-
ducting phase in the overdoped region in the high-*T _{c}*

superconductors.

**3.7. Stripes and Its Coexistence with **
**Superconductivity **

Incommensurate magnetic and charge peaks have been observed from the elastic neutron-scattering experiments in the underdoped region of the Nd-doped

**Figure 13. Energy gain per site **

###

**

**E****normal**

**E**###

**N****in the**

**SDW state as a function of hole density**

**for the three-**

**band Hubbard model. Parameters are**

**

**t**_{pp}**0.4 and**

**d**

* U*

**8 in**

**t****dp****units. From the top,**

**dp******

**

**p******

**

**d****3, 2, 1.5**

**and 1. The results are for 6 × 6, 8 × 8, 10 × 10 and 16 × 12**

**systems. Antiperiodic and periodic boundary conditions are**

**imposed in x- and y-direction, respectively. Monte Carlo****statistical errors are smaller than the size of symbols.**

**Curves are a guide to the eye [24].**

**Figure 14. Uniform SDW energy gain per site with **
**reference to the normal-state energy as a function of the **
**hole density for the three-band Hubbard model. Data are **
**from 8 × 8, 10 × 10, 12 × 12 and 16 × 12 systems for **

* p*

**

**d****2**

**** **** **. For solid symbols *** Ud*

**4 (circles),**

**

**U****d****8**

**(squares),**

**

**U**_{d}**12 (triangles) and**

**

**U**_{d}**20**

**(diamonds)**

**for**

**

**t**_{pp}**0.2 . For open symbols**

**

**U**_{d}**8 and**

**

**t**_{pp}**0 , and**

**for open squares with slash**

**

**U****d****8 and**

**

**t****pp****0.4 . The**

**lines are a guide to the eye. The Monte Carlo statistical**

**errors are smaller than the size of symbols [47].**

duction is approximately one dimensional [124]. The angle-resolved photo-emission spectroscopy measure- ments also suggested a formation of two sets of one- dimensional Fermi surface [125]. Then it has been proposed that these results might be understood in the framework of the stripe state where holes are doped in the domain wall between the undoped spin-density-wave

**Figure 15. Condensation energy per site as a function of **
**hole density for the three-band Hubbard model where **

**pp**

* t*

**0.0 ,**

****

**

_{p}****

**

_{d}**2 and**

**

**U**_{d}**8. Circles and squares**

**denote the energy gain per site with reference to the**

**normal-state energy for d-wave, ext-s wave and SDW states,****respectively. For extremely small doping rate, the extended**

**s****-wave state is more favorable than the d-wave state. Solid****symbols are for 8 × 8 and open symbols are for 6 × 6.**

**Curves are a guide to the eye.**

**Figure 16. Condensation energy per site as a function of **
**hole density for the three-band Hubbard model where **

**pp**

* t*

**0.2 ,**

****

**

_{p}****

**

_{d}**2 and**

**

**U**_{d}**8 . Circles and squares**

**denote the energy gain per site with reference to the**

**normal-state energy for d-wave and SDW states, res-****pectively. Solid symbols are for 8 × 8 and open symbols are**

**for 6 × 6. Curves are a guide to the eye.**

spots around

###

, were observed in the SC phase in the range of 0.05 *x*0.13 in the elastic and inelastic neutron-scattering experiments with LSCO [127,128,130]. The hole dependence of the incommensurability and the configuration of the spots around the Bragg spot in the SC phase indicated the vertical stripe. The neutron- scattering experiments have also revealed that a diagonal spin modulation occurs across the insulating spin-glass phase in La2–

*x*Sr

*x*CuO4 for 0.02

*x*0.05 , where a one-dimensional modulation is rotated by 45 degrees from the stripe in the SC phase. The incommensurability

versus hole density is shown in **Figure 18** sche-

matically [129,130]. The diagonal stripe changes into the vertical stripe across the boundary between the insulating and SC phase.

Let us investigate the doped system from the point of modulated spin structures [131-141]. The stripe SDW state has been studied theoretically by using the mean- filed theory [132-136]. They found that the stripe state appears when an incommensurate nesting becomes

**Figure 17. Charge and spin density as a function of the **
**distance for a striped state [50].**

**Figure 18. Schematic illustration of the incommensurability **
**versus hole density. **

favorable in the hole-doped 2D Hubbard model. When the electron correlation correlation is strong or inter- mediate, it was shown that the stripe state is more stable than the commensurate spin-density-wave state with the wave vector

###

, in the ground state of the 2D Hubbard model by using the variational Monte Carlo method [131]. It has also been confirmed by the same means that the stripe states are stabilized in the*d-p*

model [48]. The purpose of this section is to examine whether the superconductivity can coexist with static stripes in the 2D Hubbard model in a wider doping region and investigate the doping dependence of the coexisting state.

We consider the 2D Hubbard model on a square lattice. We calculate the variational energy in the coexistent state that is defined by

,

*e*
*MF*
*coexist* *P PN* *G coexist*

(37)
where *MF*

*coexist*

is a mean-field wave function. The effective mean-field Hamiltonian for the coexisting state is [105] represented by

###

†###

† ,
*ij*

*ij* *j*

*MF* *i* *i*

*ij* *ji* *ji* *j*

*H* *F* *c*

*H* *c c*

*F* *H* *c*

_{} _{} _{}

###

(38)where the diagonal terms describe the incommensurate spin-density wave state:

###

sign 1 ,

2

*i* *i*

*x* *y*

*ij* *ij* *i* *i* *ij*

*U*

*H*_{} *t* _{}*n* *m*_{} (39)
where is the chemical potential. The vertical stripe
state is represented by the charge density *ni* and the

spin density *mi* that are spatially modulated as

1 cosh *i* ,

*i*

*c*
*y* *Y*

*n*

_{} _{}

###

(40)

tanh *i* ,

*i*

*c*
*y* *Y*

*m* *m*

_{} _{}

###

(41)

where *Y* denotes the position of vertical stripes. The

amplitude is fixed by

###

*ini*

*Ne*. The off-diagonal

terms in Equation (38) are defined in terms of the *d*-wave
SC gap as

ˆ ˆ

,

*ij* *ij* *ji e*

*e*

*F*

###

(42)where ˆ*e* *x*ˆ, *y*ˆ (unit vectors). We consider two
types of the spatially inhomogeneous superconductivity:
anti-phase and in-phase defined as

###

###

###

###

ˆ

. cos ,

*i i x* *q yy* *i* *Y*

(43)

###

###

###

###

ˆ

, cos ˆ 2 ,

*i i y* *q yy* *i* *Y* *y*

(44)

###

###

###

###

ˆ

. cos ,

*i i x* *q yy* *i* *Y*

(45)

###

###

###

###

ˆ

, cos ˆ 2 ,

*i i y* *q yy* *i* *Y* *y*

(46)

respectively. Here, * q*

###

0, 2###

and is a in-commensurability given by the stripe’s periodicity in the

*y* direction with regard to the spin. The anti-phase (in-
phase) means that the sign if the superconducting gap is
(is not) changed between nearest domain walls.

The wave function 0

*coexist*

is made from the solution of the Bogoliubov-de Gennes equation represented by

###

*ij*

*j*

*ij j*

###

*i*,

*j*

*H u*_{} *F v* *E u*

###

(47)###

*ji*

*j*

*ji*

*j*

###

*i*.

*j*

*F u* *H v*_{} *E v*

###

(48) The Bogoliubov quasiparticle operators are written in the form###

†###

_{ 0 ,}

###

*i* *i* *i* *i*

*i*

*u c* *v c* *E*

###

_{}

_{} (49)

###

†###

_{0 .}

###

*i* *i* *i* *i*

*i*

*u c* *v c* *E*

###

_{}

_{} (50) Then the coexistence wave function is written as [105,142]

###

###

###

###

0 ?

1 ?

2

1 ?

0

exp 0

0 ,

*e*

*e*

*e*
*coexist* *N*

*N* _{ij}*i* *j*

*ij*

*N*

*i* *j*
*ij*
*ij*

*P*

*CP* *U V* *c c*

*C* *U V* *c c*

_{} _{}

###

###

###

(51)

for constants *C* and *C* . The calculations are
performed for the wave function 0

*coexist* *PG* *coexist*

. The

variational parameters are , *m*, *g*, *c* and *s*. The

system parameters were chosen as *t* 0.20 and
8

*U* suitable for cuprate superconductors. It has been
shown that the “anti-phase” configuration is more stable
than the “in-phase” one [105].

Here, the system parameters are *t* 0.2 and *U*8.
We use the periodic boundary condition in the *x*-di-
rection and anti-periodic one in the *y*-direction. In **Figure **
**19**, we show the total energy of the coexistent state,

*coexist*

*E* , as a function of the SC gap for the cases of
anti-phase and in-phase. The SC condensation energy

*coexist*
*E*

is estimated as 0.0008 *t* per site at the hole
density 0.125 on the 12 8 lattice with periodic
boundary condition in *x*-direction and antiperiodic one in

*y*-direction. *Ecoexist* in the coexistence state is defined

as the decrease of energy due to finite . If we use

0.5 eV

*t* , this is evaluated as 0.4 meV. The SC
condensation energy per site is shown as a function of

hole density in **Figure 20**. One finds that *Ecoexist* in the

stripe state decreases as the hole density decreases. This tendency is reasonable since the SC order is weakened in the domain of the incommensurate SDW because of the vanishingly small carrier concentration contributing the superconductivity in this domain. This behavior is con- sistent with the SC condensation energy estimated from the specific heat measurements [143].

There is a large renormalization of the Fermi surface
due to the correlation effect in the striped state [144]. We
considered the next-nearest transfer *t* in the trial
function as a variational parameter *t*. In **Figure 21**,

**Figure 19. Coexistent state energy per site ****E**_{coexist}**N**_{s}**versus ** ** for the case of 84 electrons on 12 × 8 sites with **

* U*

**8 and**

* *

**t****0.2 . Here the vertical stripe state has**

**

**8-lattice periodicity for the hole density p****0.125 . Only**

**coexist****s**

**E****N**** for the optimized gap is plotted for the in-phase **
**superconductivity.**

**Figure 20. Superconducting condensation energy per site in **
**the coexistence state as a function of the hole density **

**Figure 21. Optimized effective second neighbor transfer **
**energy ** * t t*

**as a function of U t . The system is a 16 × 16****lattice with**

* *

**t t****0.2 and the electron density 0.875.**

optimized values of *t t* _{ for the striped state are shown }
as a function of *U t* . The *t t* _{ increases as }* _{U t}*
increases. We also mention that the optimized

*t t*

almost vanishes. The renormalized Fermi surface of 0.30

*t t* _{, 0.40}_{} _{ and 0.50}_{} _{ are plotted in }_{Figure }

**22**. The system is a 16 16 lattice with *t t* 0.2 and

the electron density 0.875. As *U t* is incresed, the
Fermi surface is more deformed. We show the the
gradient of the momentum distribution function, *nk* ,

calculated in the optimized stripe state in **Figure 23**. The

brighter areas coincide with the renormalized Fermi
surface with *t t* 0.31_{ and }* _{t t}*

_{ }

_{0.0}

_{ for }

_{U t}_{}

_{8}

_{. }

The calculations for the three-band Hubbard model has
also been done taking into account the coexistence of
stripes and SC [15,106]. The energy of antiferromagnetic
state would be lowered further if we consider the incom-
mensurate spin correlation in the wave function. The
phase diagram in **Figure 24** presents the region of stable

AF phase in the plane of *t _{pp}* and

**

_{dp}**

_{p}*. For large *

_{d}*dp*

*p*

*d*, we have the region of the AF state

with an eight-lattice periodicity in accordance with the
results of neutron-scattering measurements [118,123].
The energy at *x*1 16 is shown in **Figure 25** where the

4-lattice stripe state has higher energy than that for
8-lattice stripe for all the values of *t _{pp}*.

The Bogoliubov-de Gennes equation is extended to the
case of three orbitals *d*, *p _{x}* and

*p*.

_{y}###

*H*

_{ij}_{}and

###

*Fij*are now 3

*N*3

*N*matrices. The energy of the

state with double order parameters and *m* is shown
in **Figure 26** on the 16 4 lattice at the doping rate 1/8.

The SC condensation energy per site is evaluated as
0.00016*t _{dp}*

for *U _{d}* 8,

*t*0.4 and

_{pp}* *

_{p}*2. If we use*

_{d}*t*1.5 eV [89-91], we obtain

_{dp}*E*

_{coexist}0.24 meV which is slightly smaller than and close to the value obtained for the single-band Hubbard model. We show the size dependence of the SC condensation

**Figure 22. Renormalized quasi-Fermi surface for **

* t t*

**0.3 ,**

**0.4 and**

**0.5 . The system is the same as**

**that in Figure 21.**

**Figure 23. Contour plot of ****n**_{k}** measured for the pro- **
**jected stripe state on 24 × 24 lattice with *** t t*

**0.2. The**

**electron density is 0.875.**

**Figure 25. Energy as a function of ****t****pp**** for 16 × 16 square **
* lattice at x*

**1 16. Circles, triangles and squares denote**

**the energy for 4-lattice stripes, 8-lattice stripes, and**

**commensurate SDW, respectively, where n-lattice stripe is**

**the incommensurate state with one stripe per n ladders. The**

**boundary conditions are antiperiodic in x-direction and**

**periodic in y-direction [47,106].****Figure 26. Energy of the coexistent state as a function of the **
* SC order parameter for x*

**0.125 on 16 × 4 lattice. We**

**assume the incommensurate antiferromagnetic order**

**(stripe). Parameters are **

**

_{p}**0,**

****

* *

_{d}**2,**

**

**t**_{pp}**0.4 and**

**d**

* U*

**8 in**

**t****dp****units. For solid circles the SC gap function**

**is taken as**

**i i x****,**ˆ

**cos**

###

**Q****x**###

**

**x****i***ˆ*

**x****2**

###

###

**and**

###

###

###

ˆ

* i i*

**y**

**Q****x**

**x****i****,** **cos** **, while for the open circles **

###

###

###

###

ˆ ˆ

* i i x*

**Q****x**

**x****i**

**x****,** **cos** **2** ** and ****i i****,**ˆ* y*

**cos**

###

**Q****x**###

**x****i**###

**.**

**x*** Q*

**2**

**4.**

energy for *x*0.2, 0.125 0.08333 and 0.0625 in **Figure **
**27**. We set the parameters as *p* *d* 2 and *tpp*0.4

in *tdp* units, which is reasonable from the viewpoint of

the density of states and is remarkably in accordance
with cluster estimations [89-91], and also in the region of
eight-lattice periodicity at *x*1 8. We have carried out
the Monte Carlo calculations up to 16 16 sites (768
atoms in total). In the overdoped region in the range of
0.18 *x* 0.28, we have the uniform *d*-wave pairing
state as the ground state. The periodicity of spatial

variation increases as the doping rate *x* decreases pro-
portional to 1*x*. In the figure we have the 12-lattice
periodicity at *x*0.08333 and 16-lattice periodicity at

0.0625

*x* . For *x*0.2, 0.125 and 0.08333, the results
strongly suggest a finite condensation energy in the bulk
limit. The SC condensation energy obtained on the basis
of specific heat measurements agrees well with the
variational Monte Carlo computations [99]. In general,
the Monte Carlo statistical errors are much larger than
those for the single-band Hubbard model. The large
number of Monte Carlo steps (more than _{5.0 10}_{} 7_{) is }
required to get convergent expectation values for each set
of parameters.

In **Figure 28** the order parameters *AF* and *SC*

**Figure 27. Energy gain due to the SC order parameter as a **
**function of the system size *** N_{atom}*

**3**

**N**_{s}**. Parameters are**

* p*

**0**

**** **, ***_{d}*

**2,**

**

**t**_{pp}**0.4 and**

**

**U**_{d}**8. The open circle is**

**

**for the simple d-wave pairing at the hole density x****0.2 .**

**The solid symbols indicate the energy gain of the coexistent**

**

**state; the solid circle is at x****0.125 , the solid square is at**

**

**x****

**0.08333 and the solid triangle is at x****0.0625 . The**

**diamond shows the SC condensation energy obtained on the**

**basis of specific heat measurements [99].**